Competitive Hole Transfer from CdSe
Quantum Dots to Thiol Ligands in
CdSe-Cobaloxime Sensitized NiO Films Used as
Photocathodes for H
and Leif Hammarstro
†Department of Chemistry− Ångström Laboratory, Uppsala University, Box 523, 75120 Uppsala, Sweden ‡Department of Chemistry, Qena Faculty of Science, South Valley University, 83523 Qena, Egypt
§State Key Laboratory of Fine Chemicals, DUT-KTH Joint Education and Research Center on Molecular Devices, Dalian University
of Technology, Dalian 116024, China
*S Supporting Information
ABSTRACT: Quantum dot (QD) sensitized NiO photocathodes rely on eﬃcient photoinduced hole injection into the NiO valence band. A system of a mesoporous NiO ﬁlm co-sensitized with CdSe QDs and a molecular proton-reduction catalyst was studied. While successful electron transfer from the excited QDs to the catalyst is observed, most of the photogenerated holes are instead quenched very rapidly (ps) by hole trapping at the surface thiols of the capping agent used as linker molecules. We conﬁrmed our conclusion by ﬁrst using a thiol free capping agent and second varying the thiol concentration on the QD’s surface. The later resulted in faster hole trapping as the thiol concentration increased. We suggest that this hole trapping by the linker limits the H2yield for this photocathode in a device.
Visible-light-driven H2 evolution has been attracting considerable attention from both environmental and energy points of view and also as a scientiﬁc challenge in the artiﬁcial photosynthesis community.1−7 Many systems have been employed to produce H2 from sunlight−water splitting in a similar way to the natural photosynthetic systems.4−7 In general, these systems contain a combination of light harvesting material and an active catalyst that is able to produce H2 after charge transfer from the light harvester. Therefore, a good understanding of the factors limiting photoinduced charge separation is needed to improve the catalytic activity of these systems.
Semiconductors quantum dots (QDs) like CdSe or CdS are popular sensitizers for solar energy applications including solar fuels.8,9 Here we report the photoinduced charge dynamics of both electrons and holes in an artiﬁcial system for H2evolution that contains CdSe QDs as the light harvester and the well-known molecular CoP catalyst ([CoCl(dmgH)2 (pyridyl-4-hydrophosphonate)]) (Figure 1). Both the QDs and the CoP are chemically attached to a mesoporous NiO ﬁlm via thioglycolic acid (TGA) and phosphonate groups, respectively. This system was reported recently by some of us as an eﬃcient and stable photocathode for H2production.4
CdSe QDs have been chosen as light harvesters due to their high extinction coeﬃcient, broad absorption spectrum, size-dependent tunability of the band gap, and relatively simple preparation methods. Moreover, the CoP catalyst belongs to the best transition metal complexes known to produce H2and is also easy to prepare.10 Herein, we investigate the photo-induced charge transfer dynamics upon excitation in this photocathode and ﬁnd evidence for ultrafast hole transfer reactions that compete with productive hole injection into NiO. A one-pot adsorption and reaction (OPAR) method was used to prepare the TGA-capped CdSe QDs (see the SI for more details), while the CoP catalyst was prepared according to the published procedure.11 In this Letter, we ﬁnd that the capping agent (TGA) of the QDs works as a trapping site for the photogenerated holes by using femtosecond transient absorption (TA) spectroscopy in the visible region. While the electrons are transferred from the excited QDs to the CoP catalyst as intended, most of the holes are trapped by the thiol groups and/or sulﬁde ions from the capping agent. We
Received: August 11, 2017 Accepted: October 16, 2017 Published: October 16, 2017
compared the TGA-capped OPAR-CdSe QDs with thiol-free CdSe QDs capped with oleic acid that are prepared via hot injection (HI) method as a reference sample (CdSe HI-QDs).12,13Moreover, we compared TGA-capped OPAR-CdSe QDs with successive ionic layer adsorption and reaction (SILAR-CdSe QDs), both on NiO, where the latter was reported to result in a lower catalytic activity in a device.4
Figure 2 presents steady-state absorption spectra and conﬁrms the successful attachment of the OPAR-CdSe QDs
and the CoP catalyst onto the NiO surface, (red line; see theSI
for more information about the sensitization process). Theﬁrst (1S) peak13 of CdSe QDs (black line) is unchanged by introducing the catalyst (red line). An additional absorption feature at around 400 nm is due to the CoP attachement.14
Traps in CdS and CdSe QDs are intensively discussed in the literature15,16due to their importance,17but their origin is still not very clear.18 Energetically, it has been reported that the holes can be trapped in CdSe or CdTe QDs after excitiation.18−20 This means that hole injection to a p-type
semiconductor (NiO in our system) and hole trapping processes are diﬃcult to distinguish spectroscopically where both have the same signature of charge depopulation.13,21 Herein, we will discuss the electron transfer from excited QDs to the catalyst and the self-hole trapping process by a TGA capping agent for TGA-capped CdSe QDs in a NiO/CdSe/ CoP photocathode.
Figure 3A,C presents the TA spectra of the NiO/CdSeﬁlm and NiO/CdSe/CoPﬁlm, respectively, at indicated time delays after the 400 nm excitation pulse. Generally, the spectra of excited and reduced QDs look similar,9while oxidation of QDs leads to faster recovery of the ground-state bleach (GSB) as GSB is mainly due to electron population in the conduction band.12InFigure 3A, a bleach at∼570 nm is seen due to the ﬁrst exciton absorption band of CdSe QDs (state ﬁlling of the 1S exciton).12,22On the lower-energy side of the GSB (600− 700 nm), there is strong positive absorption due to the trapped carriers, as has been reported before for CdTe QDs and CdTe/ CdS core/shell QDs.23,24 To exclude any other carrier interactions that may cause this positive absorption in our system, like biexcitonic eﬀects, we used a low pump intensity, which led to N < 1 (N is the average number of electron−hole pairs per QD).12,22
Even though the TA spectra of NiO/CdSe QD systems with and without CoP look similar, the GSB recovery dynamics of both systems are diﬀerent (Figure 3B,D, black lines). Introducing CoP catalyst accelerates the GSB recovery, meaning that the CoP catalyst consumes electrons from the excited QDs to form the reduced CoII. It was not possible to spectroscopically detect the comparably weak feature of the reduced CoP catalyst species (CoII) at around 450 nm as it was observed before25due to the positive absorption features from other species in the entire visible region, as will be discussed later, and due to its lower extinction coeﬃcient of these species.26
Comparing the GSB recovery kinetics conﬁrms the electron transfer from excited QDs to CoP catalyst.14 Figure 3B,D
Figure 1. (A) Schematic presentation of the photocathode NiO/CdSe/CoP. QDs are attached to NiO through a TGA capping agent, while CoP molecules are attached through the phosphonate group. (B) Schematic presentation of the potentials of the system components; the surface hole trap states are assigned to the thiol linkers (see the main text).
Figure 2. Steady-state UV−vis absorption spectra of the neat NiO ﬁlm (blue line), NiO/CdSe QDs ﬁlm (black line), and the full photocathode NiO/CdSe/CoP (red line).
shows the comparison of the GSB recovery (black lines) for NiO/CdSe (panel B) (τ1= 20 ps, A1= 65% andτ2= 200 ps, A2 = 34%) and NiO/CdSe/CoP (panel D) (τ1= 8 ps, A1= 77% andτ2= 65 ps, A2= 23%). The biexponential ﬁt reﬂects the typical heterogeneity of interfacial electron transfer and should not be interpreted as two distinct processes. It is well-known that the exciton lifetime of CdSe QDs (HI-QDs) is around 10− 20 ns,20while for the OPAR QDs, the exciton lifetime is very short (seeFigure S2E). The shorter exciton lifetime is due to the presence of trap states, which generally aﬀects the electron dynamics.
One important question to be answered is what is the destiny of the photogenerated holes? H2 production quantum yields under continuous irradiation are dependent on the reactions of the remaining holes in the QDs after the transfer of the electron to the catalyst.21In the ideal case scenario, as both CdSe QDs and CoP are chemically attached to NiO surface, the holes should end up in the valence band of NiO27and then migrate to the external circuit. However, we found that most of the photogenerated holes are trapped by the thiol groups and/or sulﬁde ions on a subps to ps time scale. This is seen from the rapid appearance of multiple absorption bands in the TA spectra (Figure 3A,C), where polythiol and polysulﬁde radicals are known to absorb.28−32The absorption bands remain at t > 1000 ps when all GSB is gone, which excludes assignment to a Stark eﬀect.9,14In the context of quantum dots sensitized solar cells (QDSSCs), it has been reported that hole scavenging by external scavengers,33like the sulﬁde redox couple (S2−/Sn2−)28 or sulﬁde salt as the ionic liquid,23takes place on much slower time scales (tens of ns). In our system, we observe a much faster hole trapping process (ps) with a spectroscopic signature of di- and polysulﬁde radicals.28−30 Our TA spectra are in excellent agreement with those reported for CdSe QDs on
TiO2in the presence of NaS2on a ns−μs time scale.28On one hand, capping agents are used to protect the QD surface and to prevent QD aggregation. On the other hand, TGA is the only thiol source in our system, and formation of sulﬁde radicals suggests that thiol groups are preferentially oxidized instead of the NiO valence band (Figure 1B). The rapid oxidation may be due to the direct binding of the thiol groups to the QD, while external scavengers would be sterically hindered to approach the surface by capping agents.28,33 In our case, the ultrafast radical formation may compete with desired hole transfer to NiO. To conﬁrm our conclusion that the TA signals are related to TGA oxidation, we attached the OPAR-CdSe QDs to the surface of ZrO2(noninjecting semiconductor)
in the same manner of the NiO system without the catalyst. Both samples NiO/CdSe (Figure 3A) and ZrO2/CdSe (Figure S2A) show similar TA spectra with strong positive absorption over the entire visible region due to the formation of di/polysulﬁde radicals. Moreover, we compare the TA traces of OPAR-QDs attached to ZrO2at the radical absorption peaks with the TA traces when the OPAR-QDs are attached to NiO (Figure S2B− D); the TA traces look very similar when ZrO2is replaced by NiO. This shows that a major fraction of the photogenerated holes are trapped by the thiol groups of the linker instead of being directly injected into NiO. It is diﬃcult to quantify the ratio of hole transfer to TGA vs NiO by comparing with reference samples as the TGA concentration varies between samples (TGA is added in a one-pot preparation). The radical TA signal rise is even somewhat slower on NiO than that on ZrO2 (Figure S2), which obviously cannot be explained by additional hole injection into NiO. Comparison with hole injection into NiO for QDs prepared by other methods is also questionable as the electron transfer rate can be expected to vary between diﬀerent QDs and with diﬀerent linker groups.
Figure 3. TA spectra for the NiO/CdSeﬁlm without (A) and with (C) the introduction of CoP catalyst. TA traces for NiO/CdSe ﬁlm without (B) and with (D) the introduction of CoP catalyst; black lines present the GSB recovery, and red lines present theﬁtting of the GSB recovery traces.
Furthermore, we measured the TA spectra of CdSe QDs prepared by the HI method (HI-QDs) and capped with a thiol-free capping agent, namely, oleic acid. The TA spectra did not show the spectroscopic signature of polythiol radicals and/or polysulﬁde radicals (seeFigures 3A andS1A). To conﬁrm that the formation of sulfuric radicals is due to the self-trapping of holes by the thiol groups on the QDs surface, we changed the capping agent of HI-QDs from oleic acid to TGA and attached the TGA-capped HI-QDs to a NiO ﬁlm. The resulting TA spectra of this ﬁlm indeed show similar positive absorption features on similar time scales (seeFigure S1B,C) as those for the OPAR-CdSe samples in Figure 3. This conﬁrms the involvement of the TGA capping agent in the hole trapping process. Figure 3B,D presents the traces of polythiols radical and/or polysulﬁde radical formation due to the oxidation of the thiol groups and/or sulﬁde ions by the photogenerated holes in the QDs. We also measured the TA of SILAR QDs that showed instantaneous trapping of the charge carriers upon excitation (Figure S3). This explains the poor catalytic activity of the SILAR QD devices,4 in addition to other problems like the poor loading on NiO compared to OPAR QDs.
Formation of the sulfuric radicals allows us to follow the dynamics of the photogenerated holes, but on the other hand, this trapping process competed with hole injection into NiO and is therefore likely to reduce the catalytic activity of a device. Thiol and sulfur reduction occur at mild potentials29,32,36(cf. “Hole traps” inFigure 1B), and the resulting radicals can most likely not oxidize the NiO valence band (E≈ 0.5 V vs NHE),37 as has been reported in the best-case scenario.27Although this option cannot be totally excluded in our system, we note that the radical decay kinetics on NiO and ZrO2 is essentially identical (cf.Figures 3andS2). This suggests that at least most of the holes trapped on the radicals do not lead to NiO oxidation. Instead, the rapid quenching of the QDs by TGA reduces the photocurrent and eﬃciency of H2evolution that can be achieved in a device.
Radical decay on NiO and ZrO2 is tentatively assigned to charge recombination with the reduced catalyst and/or radical reactions such as radical−radical coupling. We further note that irreversible radical reactions could make TGA a sacriﬁcial donor. This could in principle lead to high quantum yields of hydrogen generation (ΦH2) at the photocathode without the need for corresponding oxidation at the counter electrode, i.e., photochemical H2without a corresponding photocurrent. This was not the case in ref4, however, asΦH2was small and the Faradaic eﬃciency was close to 100% (and not ≫100%).4
The present study has shown that the capping agent (TGA), which protects the QDs from aggregation, itself can act as a hole trap and thus be a limiting factor for solar fuel application of QDs as a photosensitizer. Therefore, further treatments for the QDs can lead to better H2evolution eﬃciency like using thiol-free capping agents or using a core/shell structure with an optimized shell thickness38 to reduce the hole trapping probability.
*S Supporting Information
The Supporting Information is available free of charge on the
ACS Publications website at DOI: 10.1021/acsenergy-lett.7b00730.
Synthesis of CdSe QDs and NiO and complementary transient absorption data (PDF)
Mohamed Abdellah:0000-0002-6875-5886 Leif Hammarström:0000-0002-9933-9084 Notes
The authors declare no competingﬁnancial interest.
We would like to acknowledge the Knut and Alice Wallenberg Foundation (2011.0067), the Swedish Energy Agency (11674-5), the Swedish Research Council (2014-5921), and the National Natural Science Foundation of China (Nos. 21373040 and 21673028) for ﬁnancial support. Dr. Burkhard Zietz, Dr. Mélina Gilbert Gatty, Dr. Ahmed El-Zohry, and Jens Föhlinger are acknowledged for their help with the fs-TA setup. We are grateful to Minglun Cheng for preparation of the SILAR QD samples.
(1) Lubitz, W.; Tumas, W. Hydrogen: An Overview. Chem. Rev. 2007, 107, 3900−3903.
(2) Youngblood, W. J.; Lee, S.-H. A.; Maeda, K.; Mallouk, T. E. Visible Light Water Splitting Using Dye-Sensitized Oxide Semi-conductors. Acc. Chem. Res. 2009, 42, 1966−1973.
(3) Magnuson, A.; Anderlund, M.; Johansson, O.; Lindblad, P.; Lomoth, R.; Polivka, T.; Ott, S.; Stensjö, K.; Styring, S.; Sundström, V.; Hammarström, L. Biomimetic and Microbial Approaches to Solar Fuel Generation. Acc. Chem. Res. 2009, 42, 1899−1909.
(4) Meng, P.; Wang, M.; Yang, Y.; Zhang, S.; Sun, L. CdSe quantum dots/molecular cobalt catalyst co-grafted open porous NiO film as a photocathode for visible light driven H2evolution from neutral water. J. Mater. Chem. A 2015, 3, 18852−18859.
(5) McKone, J. R.; Lewis, N. S.; Gray, H. B. Will Solar-Driven Water-Splitting Devices See the Light of Day? Chem. Mater. 2014, 26, 407− 414.
(6) Esswein, A. J.; Nocera, D. G. Hydrogen Production by Molecular Photocatalysis. Chem. Rev. 2007, 107, 4022−4047.
(7) Eckenhoff, W. T.; Eisenberg, R. Molecular systems for light driven hydrogen production. Dalton Trans. 2012, 41, 13004−13021.
(8) Bang, J. H.; Kamat, P. V. Quantum Dot Sensitized Solar Cells. A Tale of Two Semiconductor Nanocrystals: CdSe and CdTe. ACS Nano 2009, 3, 1467−1476.
(9) Wu, K.; Zhu, H.; Lian, T. Ultrafast Exciton Dynamics and Light-Driven H2 Evolution in Colloidal Semiconductor Nanorods and Pt-Tipped Nanorods. Acc. Chem. Res. 2015, 48, 851−859.
(10) Kaeffer, N.; Chavarot-Kerlidou, M.; Artero, V. Hydrogen Evolution Catalyzed by Cobalt Diimine−Dioxime Complexes. Acc. Chem. Res. 2015, 48, 1286−1295.
(11) Lakadamyali, F.; Reisner, E. Photocatalytic H2evolution from neutral water with a molecular cobalt catalyst on a dye-sensitised TiO2 nanoparticle. Chem. Commun. 2011, 47, 1695−1697.
(12) Žídek, K.; Zheng, K.; Ponseca, C. S.; Messing, M. E.; Wallenberg, L. R.; Chábera, P.; Abdellah, M.; Sundström, V.; Pullerits, T. Electron Transfer in Quantum-Dot-Sensitized ZnO Nanowires: Ultrafast Time-Resolved Absorption and Terahertz Study. J. Am. Chem. Soc. 2012, 134, 12110−12117.
(13) Zheng, K.; Žídek, K.; Abdellah, M.; Zhang, W.; Chábera, P.; Lenngren, N.; Yartsev, A.; Pullerits, T. Ultrafast Charge Transfer from CdSe Quantum Dots to p-Type NiO: Hole Injection vs Hole Trapping. J. Phys. Chem. C 2014, 118, 18462−18471.
(14) Huang, J.; Mulfort, K. L.; Du, P.; Chen, L. X. Photodriven Charge Separation Dynamics in CdSe/ZnS Core/Shell Quantum ACS Energy Letters
Dot/Cobaloxime Hybrid for Efficient Hydrogen Production. J. Am. Chem. Soc. 2012, 134, 16472−16475.
(15) Jones, M.; Lo, S. S.; Scholes, G. D. Quantitative modeling of the role of surface traps in CdSe/CdS/ZnS nanocrystal photolumines-cence decay dynamics. Proc. Natl. Acad. Sci. U. S. A. 2009, 106, 3011− 3016.
(16) Wu, K.; Zhu, H.; Liu, Z.; Rodríguez-Córdoba, W.; Lian, T. Ultrafast Charge Separation and Long-Lived Charge Separated State in Photocatalytic CdS−Pt Nanorod Heterostructures. J. Am. Chem. Soc. 2012, 134, 10337−10340.
(17) Baker, D. R.; Kamat, P. V. Tuning the Emission of CdSe Quantum Dots by Controlled Trap Enhancement. Langmuir 2010, 26, 11272−11276.
(18) Utterback, J. K.; Grennell, A. N.; Wilker, M. B.; Pearce, O. M.; Eaves, J. D.; Dukovic, G. Observation of trapped-hole diffusion on the surfaces of CdS nanorods. Nat. Chem. 2016, 8, 1061−1066.
(19) Klimov, V. I. Spectral and dynamical properties of multiexcitons in semiconductor nanocrystals. Annu. Rev. Phys. Chem. 2007, 58, 635− 673.
(20) Abdellah, M.; Marschan, R.; Žídek, K.; Messing, M. E.; Abdelwahab, A.; Chábera, P.; Zheng, K.; Pullerits, T. Hole Trapping: The Critical Factor for Quantum Dot Sensitized Solar Cell Performance. J. Phys. Chem. C 2014, 118, 25802−25808.
(21) Yang, Y.; Wu, K.; Shabaev, A.; Efros, A. L.; Lian, T.; Beard, M. C. Direct Observation of Photoexcited Hole Localization in CdSe Nanorods. ACS En. Lett. 2016, 1, 76−81.
(22) Žídek, K.; Zheng, K.; Abdellah, M.; Lenngren, N.; Chábera, P.; Pullerits, T. Ultrafast Dynamics of Multiple Exciton Harvesting in the CdSe−ZnO System: Electron Injection versus Auger Recombination. Nano Lett. 2012, 12, 6393−6399.
(23) Sekhar, M. C.; Santhosh, K.; Praveen Kumar, J.; Mondal, N.; Soumya, S.; Samanta, A. CdTe Quantum Dots in Ionic Liquid: Stability and Hole Scavenging in the Presence of a Sulfide Salt. J. Phys. Chem. C 2014, 118, 18481−18487.
(24) Rawalekar, S.; Kaniyankandy, S.; Verma, S.; Ghosh, H. N. Ultrafast Charge Carrier Relaxation and Charge Transfer Dynamics of CdTe/CdS Core−Shell Quantum Dots as Studied by Femtosecond Transient Absorption Spectroscopy. J. Phys. Chem. C 2010, 114, 1460−1466.
(25) Du, P.; Schneider, J.; Luo, G.; Brennessel, W. W.; Eisenberg, R. Visible Light-Driven Hydrogen Production from Aqueous Protons Catalyzed by Molecular Cobaloxime Catalysts. Inorg. Chem. 2009, 48, 4952−4962.
(26) Bacchi, M.; Berggren, G.; Niklas, J.; Veinberg, E.; Mara, M. W.; Shelby, M. L.; Poluektov, O. G.; Chen, L. X.; Tiede, D. M.; Cavazza, C.; Field, M. J.; Fontecave, M.; Artero, V. Cobaloxime-Based Artificial Hydrogenases. Inorg. Chem. 2014, 53, 8071−8082.
(27) Liu, B.; Li, X.-B.; Gao, Y.-J.; Li, Z.-J.; Meng, Q.-Y.; Tung, C.-H.; Wu, L.-Z. A solution-processed, mercaptoacetic acid-engineered CdSe quantum dot photocathode for efficient hydrogen production under visible light irradiation. Energy Environ. Sci. 2015, 8, 1443−1449.
(28) Chakrapani, V.; Baker, D.; Kamat, P. V. Understanding the Role of the Sulfide Redox Couple (S2−/Sn2−) in Quantum Dot-Sensitized Solar Cells. J. Am. Chem. Soc. 2011, 133, 9607−9615.
(29) Asmus, K.-D. Sulfur-centered free radicals. Methods Enzymol. 1990, 186, 168−180.
(30) Asmus, K. D. Stabilization of oxidized sulfur centers in organic sulfides. Radical cations and odd-electron sulfur-sulfur bonds. Acc. Chem. Res. 1979, 12, 436−442.
(31) Chivers, T.; Drummond, I. Characterization of the trisulfur radical anion S3‑ in blue solutions of alkali polysulfides in hexamethylphosphoramide. Inorg. Chem. 1972, 11, 2525−2527.
(32) Clark, R. J. H.; Cobbold, D. G. Characterization of sulfur radical anions in solutions of alkali polysulfides in dimethylformamide and hexamethylphosphoramide and in the solid state in ultramarine blue, green, and red. Inorg. Chem. 1978, 17, 3169−3174.
(33) Huang, J.; Huang, Z.; Jin, S.; Lian, T. Exciton Dissociation in CdSe Quantum Dots by Hole Transfer to Phenothiazine. J. Phys. Chem. C 2008, 112, 19734−19738.
(34) Corani, A.; Li, M.-H.; Shen, P.-S.; Chen, P.; Guo, T.-F.; El Nahhas, A.; Zheng, K.; Yartsev, A.; Sundström, V.; Ponseca, C. S. Ultrafast Dynamics of Hole Injection and Recombination in Organometal Halide Perovskite Using Nickel Oxide as p-Type Contact Electrode. J. Phys. Chem. Lett. 2016, 7, 1096−1101.
(35) Abdellah, M.; El-Zohry, A. M.; Antila, L. J.; Windle, C. D.; Reisner, E.; Hammarström, L. Time-Resolved IR Spectroscopy Reveals a Mechanism with TiO2as a Reversible Electron Acceptor in a TiO2− Re Catalyst System for CO2Photoreduction. J. Am. Chem. Soc. 2017, 139, 1226−1232.
(36) Freedman, L. D.; Corwin, A. H. Oxidation-Reduction Potentials of Thiol-Disulfide Systems. J. Biol. Chem. 1949, 181, 601−621.
(37) Odobel, F.; Pellegrin, Y.; Gibson, E. A.; Hagfeldt, A.; Smeigh, A. L.; Hammarström, L. Recent advances and future directions to optimize the performances of p-type dye-sensitized solar cells. Coord. Chem. Rev. 2012, 256, 2414−2423.
(38) Abdellah, M.; Žídek, K.; Zheng, K.; Chábera, P.; Messing, M. E.; Pullerits, T. Balancing Electron Transfer and Surface Passivation in Gradient CdSe/ZnS Core−Shell Quantum Dots Attached to ZnO. J. Phys. Chem. Lett. 2013, 4, 1760−1765.